hybrid organic/inorganic molecular heterojunctions based on
Post on 04-Feb-2017
Embed Size (px)
Published: August 09, 2011
r 2011 American Chemical Society 3727 dx.doi.org/10.1021/nl201773d |Nano Lett. 2011, 11, 37273733
Hybrid Organic/Inorganic Molecular Heterojunctions Based onStrained NanomembranesCarlos Cesar Bof Bufon,*, Juan Diego Arias Espinoza, Dominic J. Thurmer, Martin Bauer,
Christoph Deneke,,|| Ute Zschieschang, Hagen Klauk, and Oliver G. Schmidt,
Institute for Integrative Nanosciences, IFW-Dresden, Helmholtz Strasse 20, 01069 Dresden, GermanyMaterial Systems for Nanoelectronics, TU-Chemnitz, Reichenhainer Strasse 70, 09107 Chemnitz, GermanyMax Planck Institute for Solid State Research, Heisenberg Strasse 1, 70569 Stuttgart, Germany
bS Supporting Information
The creation of organic/inorganic hybrid heterojunctionsopens the possibility for new functional elements previouslynot feasible by either component individually. Simple metal/molecule junctions have already proven highly useful for a varietyof applications.1 By adding the robustness and high carrier mobilityof an inorganic semiconductor in combination with the tailorabili-ty and processability of organic materials, novel electronic ele-ments such as hybrid resonant-tunneling diodes and field-effecttransistors2 can be realized. It is not always possible to combinematerials of different nature in a favorable way, however. Mostcommon deposition methods for metallic electrodes often havedevastating effects on ultrathin molecular layers,3 for instance.Similarly, the creation of heterojunctions consisting of well-de-fined periods of epitaxial semiconductors (such as GaAs, Si, orSiGe), which typically require high growth temperatures (2001000 C), and single organic monolayers cannot be fabricated bystandard layer-by-layer deposition techniques.4,5
Incorporating semiconductor contacts and molecular mono-layers provides an exciting alternative to further expand thehorizons of molecular electronics. First, such electrodes create anadditional degree of freedom for manipulating the charge flow inthe organic layers.6,7 Furthermore, a high level of control can beachieved by tuning the position of the Fermi level within thesemiconductor band gap via the precise adjustment of dopantmaterial and density.8 Second, the reproducibility and stability ofmolecular junctions are strongly correlated with the flatness of
the electrode.9 The use of single-crystalline semiconductors,which have surfaces intrinsically smoother than metallic layers(such as Au and Ag), is of a great advantage in this respect. Whileseveral other methods have previously been demonfor creatingsingle self-assembled molecular layers (SML), which are thensandwiched between metal and semiconductor contacts,7,1012
the fabrication and electrical characterization of semiconductor/SML/semiconductor heterojunctions using epitaxially grownmaterials is still lacking.
Self-assembly methods have been widely employed not onlyfor depositing organic monolayers13 but also for the formationof micro- and nano-objects.1416 A typical example of such anapproach is the creation of three-dimensional electronic ele-ments based on self-wound nanomembranes which can bemanu-factured in parallel on-chip.1719
Here, we present a method for preparing hybrid organic/inorganic heterojunctions using strained metal and/or semicon-ductor nanomembranes as electrodes. In this way, heterojunc-tions consisting of metal/SML/metal, semiconductor/SML/semiconductor and combinations thereof are created. In the lattercases, the semiconductor doping type and concentration can beindependently adjusted for each electrode in order to tune the
Received: May 25, 2011Revised: August 4, 2011
ABSTRACT: In this work, we combine self-assembly and top-down methods to create hybrid junctions consisting of singleorganic molecular monolayers sandwiched between metal and/or single-crystalline semiconductor nanomembrane based elec-trodes. The fabrication process is fully integrative and producesa yield loss of less than 5% on-chip. The nanomembrane-basedelectrodes guarantee a soft yet robust contact to the moleculeswhere the presence of pinholes and other defects becomesalmost irrelevant. We also pioneer the fabrication and charac-terization of semiconductor/molecule/semiconductor tunnel-ing heterojunctions which exhibit a double transition from direct tunneling to field emission and back to direct tunneling, aphenomenon which has not been reported previously.
KEYWORDS: Electronic materials and devices, molecular self-assembly, nanoscale materials, organicinorganic nanostructures,nanomembranes, strain engineering
3728 dx.doi.org/10.1021/nl201773d |Nano Lett. 2011, 11, 37273733
Nano Letters LETTER
devices electronic properties. By incorporating the self-rollingphenomenon,1416 we have developed an approach which is fullyintegrative on-chip, using well-established semiconductor pro-cessing technologies. In this way, several components can befabricated in parallel with high yield (>95%) while the activecontact area remains well below 1 m2. The strained nanomem-brane-based electrodes provide a soft yet robust contact on top ofthe SML, where damages to the molecules are minimized andshort circuits via pinholes are absent. Furthermore, we presentthe fabrication and characterization of hybrid heterojunctionshaving n- and p-doped crystalline semiconducting nanomem-branes as electrodes, contacting self-assembled monolayers(SAM). These heterojunctions exhibit electronic propertiesincluding the sequential double transition from direct tunnelingto field emission and back to direct tunneling which has notobserved for either element separately.
The simplest hybrid molecular structure proposed to date isthe metal/SML/metal junction. The main challenge for fabricat-ing such structures lies in the ability of placing themetal electrodein intimate contact with the molecular layer without damaging itsintrinsic properties or affecting the overall junction stability andreproducibility.20 The situation becomes more complex whensingle molecular layers, prepared by self-assembly for instance,are required. Here, the inevitable presence of pinholes anddefects21 over a long-range has been addressed by differentcontacting approaches,3 to enable the use of such monolayersfor device applications.22,23,25
The upper inset in Figure 1a shows a sketch of a deviceconcept to prepare metal/SML/metal heterojunctions based onrolled-up metallic nanomembranes. A detailed description of the
device fabrication is included in the Supporting Information.The rolling is caused by the self-release of a strained metallicnanomembrane by selectively etching away the underlying sacri-ficial layer. After the rolling process, a tube-shaped electrode restson top of the metallic finger, establishing an electrical connectionthrough the alkanethiol SAM (Figure 1c).
For these experiments gold (Au) layers are incorporated intothe strained metallic nanomembrane producing AualkanethiolSAM/Au junctions after rolling, as indicated in the figure. Dueto the nature of this fabrication approach, the devices can bepatterned in parallel on-chip and can even be integrated with pre-existing structures on a wafer. Figure 1b shows an SEM image ofan array of devices highlighting the excellent reproducibility ofthe fabrication process. The image was taken from a sample witha yield loss of less than 5%.
To characterize the electronic properties of the Aualkanethiol SAM/Au junctions, a positive bias is applied to afinger electrode to which the molecules are chemically bonded(inset of Figure 1a). For statistical purposes, currentvoltage(iv) traces were obtained for at least 10 devices of each alka-nethiol chain length (inset graph of Figure 1a). Similar topreviously reported work using other contacting methods,2427
the iv characteristics indicate that the current is strongly depen-dent on the SAM chain length. Since the experiments are per-formed under low bias, no significant asymmetry that mightotherwise have been caused by the different contact configura-tions (i.e., tube/CH3 physisorbed and finger-S chemisorbed) wasobserved.28 In Figure 1, the systematic change of the chain lengthfurthermore reveals direct tunneling (DT) as the dominant trans-port mechanism.24,25 As expected for coherent and nonresonant
Figure 1. (a) Differential resistance at zero bias condition (R = dV/dl|V=0) as a function of the number of CH2 groups (obtained from the ivcharacteristics displayed in the bottom inset) for Au-alkanethiol SAM/Au heterojunctions. Chemisorption and physisorption are indicated by and /,respectively. By using eq 1, was found to be 1.01( 0.05/CH2 and R0 8.9. The upper insets shows (left) the device structure before rolling and(right) after rolling. The strained layer consists of a trimetallic nanomembrane patterned on top of a sacrificial layer (details in the SupportingInformation). Once the sacrificial layer is selectively removed, the strained layer curls toward the Au finger structure (with a roughness of0.36 nm rms).After the rolling process the tube-shaped electrode rests on top of the Au finger establishing an electrical connection through the alkanethiol SAM, withchain lengths ranging from 7 to 15CH2 groups, which were previously grown on the finger surface. (b) Scanning electronmicroscope (SEM) image of anarray of devices highlighting the excellent reproducibility and parallelism of the fabrication process with a yield of at least 95%. (c) SEM image of a singleelement. The inset highlights the overlap of the tube and metallic finger electrode.
3729 dx.doi.org/10.1021/nl201773d |Nano Lett. 2011, 11, 37273733
Nano Letters LETTER
tunneling, the differential resistance (R = dV/dl|V=0) exhibits anexponential dependence on the chain length as given by25,29
R R0 expn 1
where R0 is t